Abstract
Experiments on optical and STM injection of carriers in layered MX_{2} materials revealed the formation of nanoscale patterns with networks and globules of domain walls. This is thought to be responsible for the metallization transition of the Mott insulator and for stabilization of a “hidden” state. In response, here we present studies of the classical charged lattice gas model emulating the superlattice of polarons ubiquitous to the material of choice 1T − TaS_{2}. The injection pulse was simulated by introducing a small random concentration of voids which subsequent evolution was followed by means of Monte Carlo cooling. Below the detected phase transition, the voids gradually coalesce into domain walls forming locally connected globules and then the global network leading to a mosaic fragmentation into domains with different degenerate ground states. The obtained patterns closely resemble the experimental STM visualizations. The surprising aggregation of charged voids is understood by fractionalization of their charges across the walls’ lines.
Introduction
Major anticipations for the postsilicon electronics are related to materials which demonstrate a layered structure with a possibility for exfoliation down to a few and even a single atomic layer, akin to the graphene. The latest attention was paid to oxides and particularly dihalcogenides of transition metals MX_{2} with M = Nb, Ta, Ti and X = S, Se, see e.g^{1,2}. for reviews.
These materials show a very rich phase diagram spanning from unconventional insulators of the so called Peierls and Mott types to the superconductivity^{3}. The transformations among these phases involve formation of superstructures like several types of so called charge density waves (CDW) and/or of hierarchical polaronic crystals. Recent studies of these materials fruitfully overlapped with another new wave in solid state physics. This is the science of controlled transformations of electronic states or even of whole phases by impacts of strong electric fields and/or the fast optical pumping. A super goal is to attend “hidden” states which are inaccessible and even unknown under equilibrium conditions. In relation to this article subjects, the success came recently from observations of ultrafast (at the scale of picoseconds) switching by means of optical^{4,5} and voltage^{6,7} pulses, as well by local manipulations^{8,9}. The registered ultrafast switching is already discussed as a way for new types of RAM design, see^{10} and rfs. therein.
Most challenging and inspiring observations have been done in studies by the scanning tunneling microscopy (STM) and spectroscopy (STS)^{5,8,9,11}. They have shown that the switching from an insulating to a conducting state proceeds via creation of local globules or extended networks of domain walls enforcing fragmentation of the insulating electronic crystal into a conducting mosaics of domains with different multiply degenerate ground states.
Most intriguing observations have been done upon very popular nowadays layered material 1T − TaS_{2} which is a still enigmatic “polaronic Wignercrystalline Mott insulator”. The rich phase diagram of 1T − TaS_{2} includes such states as incommensurate, nearly commensurate, and commensurate CDWs which unusually support also the Mott insulator state for a subset of electrons. Recently, new longlived metastable phases have been discovered: a “hidden” state created by laser^{4,5} or voltage^{6,7} pulses, and a most probably related “metallic mosaic” state created locally by STM pulses^{8,9}.
1T − TaS_{2} is a narrowgap Mott insulator existing unusually on the background formed by a sequence of CDW transitions which have gaped most of the Fermi surface of the high temperature metallic (with 1 electron per Ta site) parent phase^{2}. Incomplete nesting leaves each 13th electron ungaped which in a typical CDW would give rise to a pocket of carriers. Here, each excess carrier is selftrapped by inwards displacements of the surrounding atomic hexagon (forming the “David star” unit) which gives rise to the intragap local level accommodating this electron. Exciting the selftrapped electron from the intragap level leads to a partial relaxation of deformation, the David star levels out in favor of a void in the crystal of polarons. The charged voids are expected to arrange themselves into a Wigner crystal subjected to constraints of commensurability and packing with respect to the underlying structure.
A major question arises: why and how the repulsive voids aggregate into the net of walls leaving microcrystalline domains inbetween? In this paper, we answer this and related questions by modeling the superlattice of polarons upon the 2D triangular basic lattice of all Ta atoms by a classical charged lattice gas with a screened repulsive Coulomb interaction among the particles. The external pulse injecting the voids was simulated by introducing a small random concentration of voids reducing the particles concentration ν below the equilibrium ν_{0} = 1/13 (some other experimentally relevant concentrations are briefly described in the Supplementary Material, Sec. IV). The subsequent evolution of the system, including the passage through the thermodynamic first order phase transition, was studied by means of the Monte Carlo simulation. Surprisingly, this minimalistic model is already able to capture the formation of domain walls in a close visual resemblance with experimental observations and also to explain the effect qualitatively as an intriguing result of the charge fragmentation.
It is worth noticing that the described here phenomena can be viewed in a more general perspective of “nanonetworks” which notion unifies observations on nanosize aggregates in biological, physics and chemistry and the mathematical graphs theory, see the reviews^{12,13}.
The model
We model the system of polarons by a lattice gas of charged particles on a triangular lattice. Each particle represents the selftrapped electron in the middle of the David star, thus the effective charge is −e, which in average is compensated by the static uniform positive background.
The external pulse is simulated by a small concentration of randomly seeded voids reducing the particles’ concentration below the equilibrium: ν = ν_{0} − δν. The interaction of polarons located at sites i, j is described by an effective Hamiltonian H = ∑_{i,j}U_{ ij }n_{ i }n_{ j } with repulsive interactions U_{ ij }. Here the sum is over all pairs of sites i ≠ j; n_{ i } = 1 (or 0) when particle is present (or absent) at the site i, and we choose U_{ ij } as the screened Coulomb potential
where U_{0} = e^{2} exp(−a/l_{ s })/a is the Coulomb energy of interaction of particles at neighboring sites in the Wigner crystal state with the distance \(a=\sqrt{13}b\) between them (b is the lattice spacing of the underlying triangular lattice, Fig. 1a), l_{ s } is the screening length. The screening length comes from a small density of states at the Fermi level^{8}. Considering the delocalized electrons as a 2D Fermi gas, we get \({l}_{s}\sim \sqrt{\pi \mathrm{/2}{d}_{3}{r}_{B}}\) where d_{3} is the interplane distance and r_{ B } is the effective Bohr radius.
Superlattice and its charged defects
In the ground state, the charged particles living on the triangular lattice tempt to arrange themselves in also the triangular superlattice, which is closepacked and most energetically favorable in 2D^{14} (with some notable exceptions for more exotic potentials^{15}). Figure 1a illustrates, in accordance with all structural experiments, that it can be done indeed, with the superlattice vectors inclined by ±13.9° with respect to the host one–the chirality sign determining the mirror symmetry breaking (the right chirality was chosen to be shown.) The most important for us is the translational symmetry breaking leaving 13fold degeneracy with respect to positioning of the David stars’ central atoms at the host sites. The total degeneracy is 26fold. Until recently it was thought that the two mirrorsymmetric phases do not not coexist within a given sample experimentally^{16} and in the modeling for the sufficiently slow cooling rates (probably because of the high energy of the corresponding twinning wall). However, recent experiments^{17} and the numerical modeling for the fast cooling rates indicate that the two chiral phases can coexist–see Supplementary Sec. V for the details.
The David star, taken as a symmetric unit cell, contains three nonequivalent cites: the central one, the 6 nearest neighbors and 6 nextnearest neighbors. We shall associate the polaron location with the central site while basic allowed defects correspond either to its elimination (the void as the point defect) or to its replacement to one of NN or NNN positions (the domain walls as line defects). The simplest lattice defect is a void or a “polaronic hole” (Fig. 1b) which is formed when the electron from the intragap level is taken away or excited to the conduction band and soon the associated lattice distortions are partially released. The single void has the relative charge +e (keeping in mind the background neutralizing charge) and the Coulomb selfenergy of the order \({E}_{void}\simeq {e}^{2}/a\). While the void is a particular manifestation of a general notion of vacancies in crystals, in our case there can be also a specific topologically nontrivial defect–the domain wall separating domains with a different 13fold positional degeneracy of the ground state (Fig. 2). The domain wall crosssection resembles the discommensuration known in CDW systems^{18}.
Experimentally, the lattice defects can be introduced via external pulses, by impurity doping or by the field effect. For example, a laser or STM pulse can excite the Mottband electrons residing in the centers of the David star clusters, creating an ensemble of voids. Since the voids are charged objects, then at first sight they should repel each other and form a Wigner crystal themselves. But our modeling consistent with the experiment shows that the voids rather attract one another at short distances and their ensemble is unstable towards formation of domain walls’ net. Qualitatively, this instability can be understood from the following argument. Compare energies of the isolated void and of the domain wall segment carrying the same charge. The minimal charge of domain wall per the translation vector a_{1} is +e/13 (Fig. 2a), and the energy of the wall’s segment carrying the charge +e can be estimated as for a uniformly charged line:
For moderate screening lengthes l_{ s }, it is lower than the void’s selfenergy E_{ void }, making energetically favorable to decompose the voids into fractionallycharged domain walls. The local effects beyond our model can also favor domain walls with other charges: for the singlestep +1e/13 domain wall there are anomalous sites where David stars intersect (Fig. 2a) which raises its energy and can make the doublestep +2e/13 domain walls (Fig. 2b) to be energetically favorable. The same qualitative arguments can be applied to the case of doping by interstitials rather then voids.
Numerical modeling
We simulated the cooling evolution of the classical lattice gas with the interaction potential (1) via Metropolis Monte Carlo algorithm (see Methods). We perform slow cooling from T = 0.055U_{0}, which is above the detected ordering phase transition (see below), down to T = 0.01U_{0} with a step ΔT = −0.0001U_{0}, reaching either a ground state or a very close in energy metastable state. Below we, first, consider undoped systems (where particles concentration ν is exactly ν_{0} = 1/13), and then systems doped by voids (with ν = ν_{0} − δν ≡ ν_{0}(1 − ν_{ voids }), where ν_{ voids } = δν/ν_{0} is the voids’ concentration). Results for another sign of doping are briefly presented in the Supplementary Material, Sec. IV.
Undoped system
As a reference system we chose the sample with 91 × 104 sites with the total a number of particles N_{ p } = 728, which corresponds to the concentration ν_{0} = 1/13.
On cooling, the orderdisorder phase transition takes place at T_{ c } ≈ 0.042U_{0}, below which the triangular superlattice is formed confirming the expectations for the Wigner crystal. Temperature dependencies of the order parameter \(M=\sqrt{13\sum {({m}_{i}1/13)}^{2}/12}\), where m_{ i } is the fraction of particles at the ith sublattice (Fig. 3a) and of the mean value of energy per particle (Fig. 3b) indicate that the transition is of the first order. The insets in the Fig. 3a show a plenty of defects just above T_{ c }, while only two displaced positions are left just below T_{ c }.
On heating, the orderdisorder phase transition takes place at T ≈ 0.049U_{0}, which agrees with our mean field analysis (see Supplementary Sec. III). With increasing l_{ s } the temperature hysteresis and the tendency to overcooling become more pronounced. An overcooling or even freezing into in a glass state feature is known for electronic systems with either a frozen disorder or a Coulomb frustrations^{19}; however in the present model these both factors are absent – the effect is presumably due to only the longrange Coulomb interactions under the lattice constraints.
Doped system
We emulate the doping (the charge injection) by seeding voids at random places and following the subsequent evolution. By global characterizations like those in Fig. 3, the orderdisorder transition is preserved, while at a lower temperature. But locally the new mosaic ground state with the net of domain walls is formed as we will demonstrate below.
Seeding at T < T_{ c } a small number of voids, down to two defects per sample, we observe that the singlevoid states are unstable with respect to their binding and progressive aggregation. Seeding more voids initiates their gradual coalescence into a globule of interconnected segments of domain walls. The resulting globule performs slowly a random diffusion over the sample while keeping closely its optimal shape and the structure of connections (the Supplementary Video of the system evolution under cooling and its description are presented in Supplementary Sec. I).
Despite it is not necessary to go through the orderdisorder transition to obtain the globule structures–the seeding of voids can be performed within the ordered phase, but the equilibration times become much longer in this case. Therefore in order to obtain the lowtemperature configurations for the doped systems we use the same strategy as for undoped ones: we cool down the system starting from the disordered state at T > T_{ c }.
Figure 4a shows the lowT configuration of a 156 × 182 system, where initially N_{ p } = 2184 of particles (with the the corresponding concentration of voids ν_{ voids } ≈ 0.9%) were randomly seeded and then the system was slowly cooled from T = 0.055U_{0} > T_{ c } down to T = 0.01U_{0}. In spite of the initial random distribution of particles over the whole sample, finally the voids aggregate into a single globule immersed into a connected volume of the unperturbed crystal. We compare the results of our modeling in Fig. 4a with the experimental picture in Fig. 4b^{8}. Similar patterns have been observed also in other experiments^{6}: (Fig. 3 of the supplement) and^{9} (Fig. 1). By adding the particles to the obtained globule configuration, we can reverse the doping and anneal the system at T = 0.04U_{0} < T_{ c }. Then the globule gets erased and the system relaxes pretty fast to the uniform state, which takes \(\sim 5\times {10}^{6}\) steps, see Supplementary Sec. II for the details.
With a further increase of doping, the globule size grows over the whole sample, and finally the branched net of domain walls divides the system into the mosaics of randomly shaped domains (Fig. 5a,c). The comparison of the modeling with the experiment on injection by the STM pulses is shown between panels (a) and (b) in Fig. 4, between panels (a) and (b), (c) and (d) in Fig. 5. The figures visualize a spectacular resemblance of our modeling with results from several STM experiments exploiting either the optical switching to the hidden state^{5} or the pulses from the STM tip^{8,9}. Note that “irregular honeycomb network” structures were predicted for incommensurate phase of krypton on graphite with ν_{0} ≈ 1/3 and shortrange interaction^{20}, but with more topological restrictions than here.
Discussion and Conclusions
Our simulations have shown an apparently surprising behavior: some effective attraction of voids develops from the purely repulsive Coulomb interactions. The coalescence of single voids starts already at their small concentration. For several voids seeded, we observe a gradual fusion of point defects into the globule of the domain walls. Increasingly branched net develops with augmenting of the voids concentration.
That can be understood indeed by noticing that the walls formation is not just gluing of voids but their fractionalization. The domain wall is fractionally (q = ν_{0}e) charged per its crystalunit length, thus reducing the Coulomb selfenergy in comparison with the integercharged single void. Being the charged objects, the domain walls repel each other, but as topological objects they can terminate only at branching points, thus forming inplane globules. Their repulsion at adjacent layers meets no constraints, hence the experimentally observed alternation of the walls’ patterns among the neighboring layers^{5,8,9}.
A similar while simpler doping induced phase transition to the state patterned by charged domain walls was predicted for quasi1D electronic systems with 2fold degeneracy from the Peierls effect of the spontaneous dimerization, see^{21}.
Our modeling can be straightforwardly extended to other values of concentration ν_{0}: like ν_{0} = 1/3 which is the minimal value where the pattern formation appears with qualitatively similar to the presented here results (see Supplementary Sec. IV) and corresponding, for example, to the \(\sqrt{3}\times \sqrt{3}\) surface CDW observed in the lead coated germanium crystal^{22}. For another experimentally known case of 2H − TaSe_{2} where ν_{0} = 1/9 the modeling results are quite different: in some doping range we see a “stripe” phase (see Supplementary Sec. IV), which indeed was experimentally observed in this material^{23}. The exception of the case ν_{0} = 1/9 is rather natural, because here the basis vectors of the superlattice and of the underlying triangular lattice are parallel to each other, which allows for the existence of neutral elementary domain walls.
It is also possible to study the doping by electrons by seeding the interstitials rather than voids; here the new David stars substantially overlap with their neighbors giving rise to stronger lattice deformations, which may require for a more complicated model. The fragmentation with formation of walls is always confirmed while details of patterns can differ (see Supplementary Fig. 9).
The encouraging visual correspondence of our pictures with experimentally obtained patterns in different regimes of concentrations ensures a dominant role of the universal model.
Methods
For numerical simulation of the classical lattice gas with interaction potential (1) we employed the Metropolis Monte Carlo method. We used the screening parameter l_{ s } = 7.2b ≈ 2a and truncated the interactions to zero for sufficiently large interparticle distances–outside the hexagon with the side 40b (we also performed the modeling for l_{ s } = 4.5b ≈ 1.25a with qualitatively similar results, see Supplementary Materials). At each temperature we performed ~5–10 millions of Monte Carlo steps depending on the numerical experiment. Temperature was linearly lowered from T = 0.055U_{0} down to T = 0.01U_{0} with a step ΔT = −0.0001U_{0}. The following system sizes and numbers of particles were chosen: size 91 × 104 and N_{ p } = 728 for undoped system; size 156 × 182 and N_{ p } = 2184, ν_{ voids } ≈ 0.9% for the globule system (Fig. 4a); size 142 × 168 and N_{ p } = 1758, ν_{ voids } ≈ 1.9% for the net system (Fig. 5a,c). Periodic rectangular boundary conditions were imposed.
Data availability
The datasets generated during and analysed during the current study are available from the corresponding author on reasonable request.
References
Manzeli, S., Ovchinnikov, D., Pasquier, D., Yazyev, O. V. & Kis, A. 2D transition metal dichalcogenides. Nat. Rev. Mater. 2, 17033 (2017).
Rossnagel, K. On the origin of chargedensity waves in select layered transitionmetal dichalcogenides. J. Phys. Condens. Matter 23, 213001 (2011).
Sipos, B. et al. From Mott state to superconductivity in 1T − TaS_{2}. Nat. Mater. 7, 960–965 (2008).
Stojchevska, L. et al. Ultrafast switching to a stable hidden quantum state in an electronic crystal. Science 344, 177–180 (2014).
Gerasimenko, Ya. A., Vaskivskyi I. & Mihailovic, D. Long range electronic order in a metastable state created by ultrafast topological transformation. arXiv:1704.08149 (2017).
Vaskivskyi, I. et al. Fast electronic resistance switching involving hidden charge density wave states. Nat. Commun. 7, 11442 (2016).
Yoshida, M. et al. Controlling chargedensitywave states in nanothick crystals of 1T − TaS_{2}. Scientific Reports 4, 7302 (2014).
Ma, L. et al. A metallic mosaic phase and the origin of Mottinsulating state in 1T − TaS_{2}. Nat. Commun. 7, 10956 (2016).
Cho, D. et al. Nanoscale manipulation of the Mott insulating state coupled to charge order in 1T − TaS_{2}. Nat. Commun. 7, 10453 (2016).
Svetin, D., Vaskivskyi, I., Brazovskii, S. & Mihailovic, D. Threedimensional resistivity switching between correlated electronic states in 1T − TaS_{2}. Scientific Reports 7, 46048 (2016).
Cho, D. et al. Correlated electronic states at domain walls of a Mottchargedensitywave insulator 1T − TaS_{2}. Nat. Commun. 8, 392 (2017).
Boccaletti, S., Latora, V., Moreno, Y., Chavez, M. & Hwang, D.U. Complex networks: Structure and dynamics. Physics Reports 424, 175–308 (2006).
Zivkovic, J. & Tadic, B. Nanonetworks: The graph theory framework for modeling nanoscale systems. NanoMMTA 2, 30–48 (2013).
Bonsall, L. & Maradudin, A. A. Some static and dynamical properties of a twodimensional Wigner crystal. Phys. Rev. B 15, 1959 (1977).
Jagla, E. A. Minimum energy configurations of repelling particles in two dimensions. Journ. Chem. Phys. 110, 451–456 (1999).
Shiba, H. & Nakanishi, K. In “Structural Phase Transitions in Layered Transition Metal Compounds”, ed. K. Motizuki (D. Reidel Publishing Company, Dordrecht, 1986).
Gerasimenko, Ya. A. & Mihailovic, D. (private communications).
McMillan, W. L. Theory of discommensurations and the commensurateincommensurate chargedensitywave phase transitions. Phys. Rev. B 14, 1496–1502 (1976).
Mahmoudian, S., Rademaker, L., Ralko, A., Fratini, S. & Dobrosavljevic, V. Glassy Dynamics in Geometrically Frustrated Coulomb Liquids without Disorder. Phys. Rev. Lett. 115, 025701 (2015).
Villain, J. Commensurateincommensurate transition of krypton monolayers on graphite: a low temperature theory. Surface Science 97, 219–242 (1980).
Karpov, P. & Brazovskii, S. Phase transitions in ensembles of solitons induced by an optical pumping or a strong electric field. Phys. Rev. B 94, 125108 (2016).
Carpinelli, J. M., Weitering, H. H., Plummer, E. W. & Stumpf, R. Direct observation of a surface charge density wave. Nature 381, 398–400 (1996).
Fleming, B. M., Moncton, D. E., McWhan, D. B. & DiSalvo, F. J. Broken Hexagonal Symmetry in the Incommensurate ChargeDensity Wave Structure of 2H − TaSe_{2}. Phys. Rev. Lett. 45, 576 (1980).
Acknowledgements
The authors are grateful to Ya.A. Gerasimenko, D. Mihailovich, E. Tosatti and H.W. Yeom for helpful discussions. We acknowledge the financial support of the Ministry of Education and Science of the Russian Federation in the framework of Increase Competitiveness Program of NUST MISiS (N K32017033). SB acknowledges funding from the ERC AdG 320602 “Trajectory”. PK acknowledges the support of the Arconic Foundation. Image source for Figs 4(b), 5(b,d) is^{8}; use permitted under the https://creativecommons.org/licenses/by/4.0/Creative Commons Attribution License CC BY 4.0; the images were cropped and rotated.
Author information
Authors and Affiliations
Contributions
S.B. and P.K. together formulated the theoretical concept, designed the model, analyzed results, and wrote the paper; P.K. performed the numerical computations. Correspondence and requests for materials should be addressed to P.K.
Corresponding author
Ethics declarations
Competing Interests
The authors declare no competing interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Electronic supplementary material
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Karpov, P., Brazovskii, S. Modeling of networks and globules of charged domain walls observed in pump and pulse induced states. Sci Rep 8, 4043 (2018). https://doi.org/10.1038/s41598018223087
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s41598018223087
This article is cited by

Lightinduced dimension crossover dictated by excitonic correlations
Nature Communications (2022)

A timedomain phase diagram of metastable states in a charge ordered quantum material
Nature Communications (2021)

Multivalley Free Energy Landscape and the Origin of Stripe and QuasiStripe CDW Structures in Monolayer MX2 Compounds
Scientific Reports (2020)

Quantum jamming transition to a correlated electron glass in 1TTaS2
Nature Materials (2019)

Intertwined chiral charge orders and topological stabilization of the lightinduced state of a prototypical transition metal dichalcogenide
npj Quantum Materials (2019)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.